Upcoming SlideShare
×

# Friction – etiology & management in straight wire technique /certified fixed orthodontic courses by Indian dental academy

1,899 views

Published on

The Indian Dental Academy is the Leader in continuing dental education , training dentists in all aspects of dentistry and offering a wide range of dental certified courses in different formats.

Indian dental academy provides dental crown & Bridge,rotary endodontics,fixed orthodontics,
Dental implants courses.for details pls visit www.indiandentalacademy.com ,or call
00919248678078

2 Likes
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
• Be the first to comment

Views
Total views
1,899
On SlideShare
0
From Embeds
0
Number of Embeds
1
Actions
Shares
0
22
0
Likes
2
Embeds 0
No embeds

No notes for slide

### Friction – etiology & management in straight wire technique /certified fixed orthodontic courses by Indian dental academy

1. 1. Friction – Etiology & Management in SWA www.indiandentalacademy.com
3. 3. One of the most common methods of translating a tooth orthodontically - sliding mechanics. Mesiodistal tooth movement - by guiding a tooth along a continuous arch wire with the use of an orthodontic bracket. Disadvantage - friction - resist the movement. www.indiandentalacademy.com
4. 4. Friction is defined as a force that retards or resists the relative motion of two objects in contact, and its direction is tangential to the common boundary of the two surfaces in contact. Frictional force - 2 sliding surfaces α to the force - surfaces are pressed together. Ffr = u × F. The value of u (the coefficient of friction) www.indiandentalacademy.com
5. 5.  Static Frictional forces - smallest force needed to start a motion of solid surfaces with respect to each other.  Kinetic frictional force - force needed to resist the sliding motion of one solid object over another at a constant speed. www.indiandentalacademy.com
6. 6. Several variables - directly or indirectly contribute - friction – b/w - bracket & wire; They are:  Arch wire.  Material.  Cross-sectional shape/size.  Surface texture.  Stiffness. www.indiandentalacademy.com
7. 7.  Ligation of arch wire to bracket.  Ligature wires.  Elastomerics.  Bracket.      Material. Slot width and depth. First order bend (in-out). Second order bend (angulation). Third order bend (torque). www.indiandentalacademy.com
8. 8.  Orthodontic appliance.  Interbracket distance.  Level of bracket slots between adjacent teeth.  Forces applied for retraction.  Intraoral variable.     Saliva. Plaque. Acquired pellicle. Corrosion. www.indiandentalacademy.com
9. 9.  Static frictional force = coefficient of static friction x resultant normal force;  Kinetic frictional force = coefficient of kinetic friction x resultant normal force.  The coefficients of static and kinetic friction, generally having magnitudes between zero and one,  depend upon -relative roughness of the contacting surfaces. www.indiandentalacademy.com
10. 10. Prososki etal (AJO-1991) states that surface roughness influences friction most directly when  dry, unlubricated sliding occurs or when only meager lubrication is present.  geometry of roughness,  orientation of roughness features, and  relative hardness of the two contacting surfaces. Friction tends to be highest for very rough or very smooth surfaces. www.indiandentalacademy.com
11. 11.  Sliding mechanics- biologic tissue response and tooth movement - applied forces overcome the friction at the bracket-wire interface.  High levels of bracket-wire friction may result in  binding of the bracket  little or no tooth movement.  binding of an anterior tooth under retraction  loss of anchorage. The most desirable and ideal situation, - little or no friction - b/w bracket and wire. www.indiandentalacademy.com
12. 12.  Proffit etal considers frictional resistance in orthodontic appliance to be multifactorial,  It is α force with which the contacting surfaces are pressed together  Affected by the nature of the surface at the interface  Independent of the apparent area of contact www.indiandentalacademy.com
13. 13.  role of asperities (limited number of small spots at the peak of surface irregularities) - contributing factor.  These elevated areas carry the entire load between two surfaces and may undergo plastic deformation with appropriate force.  Applied load determines the true contact area. www.indiandentalacademy.com
14. 14.  coefficient of friction is  α shear strength of the junction &  1/ α yield strength of the material.  The interlocking of large and pointed asperities or ‘plowing’ of asperities into opposing surfaces -  friction. www.indiandentalacademy.com
15. 15. Arch wire:  Material: Garner et al (AJO-1986) – found significantly larger frictional force with beta-titanium and nitinol when compared with stainless steel. Differences in surface smoothness - account for the differences in friction. www.indiandentalacademy.com
16. 16. SEM - SS NiTi www.indiandentalacademy.com
17. 17. Beta - Titanium www.indiandentalacademy.com
18. 18. Drescher et al - SEM study - between diverse wire materials.  SS and Elgiloy - smooth surface texture,  NiTi, TMA, - extensive surface roughness.  Surface texture - friction magnitude in edgewise mechanics.  Effective force has to increase by twofold (stainless steel) to sixfold (TMA) to overcome bracket-to-wire friction. www.indiandentalacademy.com
19. 19.  Tidy DC - fixed appliance in vitro to simulate tooth movement in a previously aligned arch.  Nitinol and TMA (beta-titanium) >frictional forces -2x & 5x – of SS.  SS arch wires may be used in preference to nitinol or TMA arch wires to reduce the friction in sliding mechanics. www.indiandentalacademy.com
21. 21. Kapila et al (AJO- 1990) greater magnitude and more frequent variation in frictional forces per unit distance of bracket travel with NiTi and ß-Ti wires than with SS or Co-Cr wires.  Higher mean frictional forces - NiTi and ß-Ti wires.  surface roughness of these alloys > SS or Co-Cr in SS brackets www.indiandentalacademy.com
22. 22.  Archwire Dimension:  Tidy found that wire dimension and slot size had little effect on friction.  Vaughan etal - The frictional forces  with   rectangular wire than with round wire, and  wire size   frictional force.  Pizzoni - friction occurring in sliding mechanics as being influenced by the bracket design, wire material and wire cross section.  He concluded that round wires have lesser friction than rectangular wires, www.indiandentalacademy.com
23. 23.  Kapila et al(AJO 1990) - Stainless steel, Co-Cr, and ß-Ti wires ↑ bracketwire friction with increase in wire size. Increase in size of NiTi wires - no significant effect on - friction between bracket and wire – in 0.018 inch narrow single br.. www.indiandentalacademy.com
24. 24.  Surface properties:  Ryan et al- (AJO 1997) - effects of ion implantation on the rate of tooth movement.  ion-implanted wires - > movement than their untreated counterparts.  The ion-implantation process -  stress fatigue and hardness of the material  the friction. www.indiandentalacademy.com
25. 25.  Brackets: Drescher et al -study found narrow brackets to intensify friction by enhancing tipping movements. This implies a preference for the use of medium or wide brackets in arch-guided tooth movement, particularly in cases in which excessive mesiodistal tooth translation is required www.indiandentalacademy.com
26. 26.  Andreasen and Quevodo, - study to evaluate the frictional forces in the 0.022 X 0.028” edgewise bracket system.    Multiple round and rectangular SS wires, brackets of three different widths, four bracket wire angulations. both wet and dry conditions  Tipping the bracket &larger wires -  friction,  Bracket width & wet and dry conditions were found to be insignificant www.indiandentalacademy.com
27. 27.  Tidy studied the effect of load, bracket width, slot size, arch wire size, and material.  The forces acting on the surface of the tooth root were simulated by a single equivalent force acting at the center of resistance of the root. The couple produced by the two-point contact with the arch wire counters the moment of this force about the arch wire. www.indiandentalacademy.com
29. 29.  The movable bracket was fitted with a 10 mm power arm - weights - hung –force acting at the center of resistance of the tooth root. The length of the power arm - distance from the slot to the center of resistance of a typical canine tooth.  The movable bracket was suspended from the load cell of the testing machine, while the baseplate moved downward with the crosshead on which it was mounted. www.indiandentalacademy.com
31. 31. Friction α applied load and 1/ α bracket width. The friction was greatest for narrow brackets. Wide brackets and stainless steel arch wires may be used in preference to nitinol or TMA arch wires to reduce the friction in sliding mechanics. www.indiandentalacademy.com
32. 32.  Kapila et al.- investigated –  Frictional properties of Stainless steel (SS), cobalt- chromium (Co-Cr), nickel-titanium (NiTi), and βtitanium (β -Ti) wires of several sizes were tested in narrow single (0.050-inch), medium twin (0.130inch) and wide twin (0.180-inch) stainless steel brackets in both 0.018 and 0.022-inch slots.  frictional force  - wider brackets  Due to the higher force of ligation - the greater stretching of elastic ligatures on wider brackets. www.indiandentalacademy.com
33. 33. Vaughan et al –  Overall friction of sintered stainless steel brackets 40% to 45% < conventional cast stainless steel brackets.  Pratten et al- frictional resistance of ceramic and SS brackets + SS and NiTi wire. Ceramic brackets  frictional resistance than SS brackets when used in combination with either SS or NiTi arch wires. www.indiandentalacademy.com
34. 34.  Dickson etal- experimental polycrystalline ceramic bracket with a SS insert and compared conventional & SS bracket.  The exptl. bracket -  frictional resistance and the ceramic bracket - 0˚ angulation. No sig. diff. between the two ceramic brackets at 10˚,  frictional resistance than SS bracket. Stainless Steel insert slot - experimental bracket behave more like a stainless steel bracket rather than a conventional ceramic bracket. www.indiandentalacademy.com
35. 35.  Madhav.M and Jyothindra Kumar compared the frictional properties and debonding characteristics of gold inserted slot Luxi™ bracket system and stainless steel inserted Clarity™ bracket system and compared them with stainless steel Gemini™ bracket.  Metal inserted ceramic brackets - frictional properties as good as stainless steel brackets.  Luxi™ - least kinetic friction  Clarity™ bracket - highest value, of the three bracket systems evaluated for both 50 gms and 100 gms load. www.indiandentalacademy.com
36. 36.  Ligation.  Edwards et al- ligation techniques - on the static frictional resistance of stainless steel brackets and archwires - dry and wet conditions.  No significant differences in frictional resistance were found between conventionally tied elastomeric modules and stainless steel ligatures. Teflon-coated ligatures - lowest frictional forces. www.indiandentalacademy.com
37. 37.  David etal- ( AO – 95) - static frictional resistances between  Teflon- coated stainless steel and clear elastomeric ligatures –with   SS, polycrystalline ceramic and single crystal ceramic 0.022-inch slot brackets, SS and NiTi archwires, 0.018 inch and 0.016 × 0.022 inch.  Friction was measured in the dry state at bracket- archwire angulations of 0, 5, 10, and 15 degrees.  Teflon-coated SS ligatures - friction than elastomeric ligatures regardless of bracket type, archwire type, or bracket-archwire angulation. www.indiandentalacademy.com
38. 38.  Self ligation. SPEED ApplianceSpring-loaded, Precision, Edgewise, Energy, and Delivery, all of which describe features of the design. www.indiandentalacademy.com
39. 39. Berger (AJO – 1990) ↓ force - required to move rectangular steel or round braided arch wires - a standard distance self-ligation SPEED bracket < the elastomeric and the steel-tie ligated "A"-Company and American Orthodontics bracket systems. www.indiandentalacademy.com
40. 40.  Activa brackets -fully programmed preadjusted brackets that were introduced in 1986- Irwin Pletcher.  The arch wire -retained - resilient clip retaining groove gingival to the arch wire.  The friction is < elastomeric rings and conventional brackets. www.indiandentalacademy.com
41. 41.  Shivapuja etal (AJO1994) – Compared three self-ligating bracket systems to conventional SS brackets and ceramic brackets + polyurethane elastomeric and SS tie wire ligation.  Self-ligating bracket systems -  frictional resistance,  chairtime for arch wire removal and insertion. www.indiandentalacademy.com